#------------------------------------------------------------------------------
#$Date: 2017-05-06 01:12:10 +0300 (Sat, 06 May 2017) $
#$Revision: 196457 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/25/7042557.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7042557
loop_
_publ_author_name
'He, Zhangzhen'
'Guo, Wenbin'
'Cui, Meiyan'
'Tang, Yingying'
_publ_section_title
;
 Synthesis and magnetic properties of new tellurate compounds Na4MTeO6 (M
 = Co and Ni) with a ferromagnetic spin-chain structure.
;
_journal_issue                   15
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5076
_journal_page_last               5081
_journal_paper_doi               10.1039/c6dt04750e
_journal_volume                  46
_journal_year                    2017
_chemical_formula_moiety         'Co O6 Te, 4(Na) '
_chemical_formula_sum            'Co Na4 O6 Te'
_chemical_formula_weight         374.49
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           13
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2016-12-13 deposited with the CCDC.
2017-03-21 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 109.470(14)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   5.677(5)
_cell_length_b                   9.524(7)
_cell_length_c                   5.485(4)
_cell_measurement_reflns_used    854
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4662
_cell_measurement_theta_min      2.1384
_cell_volume                     279.6(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.980
_diffrn_measured_fraction_theta_max 0.980
_diffrn_measurement_device_type  'Saturn724+ (2x2 bin mode)'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0393
_diffrn_reflns_av_sigmaI/netI    0.0410
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            2033
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_diffrn_reflns_theta_min         4.28
_diffrn_standards_number         669
_exptl_absorpt_coefficient_mu    8.461
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6929
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            purple
_exptl_crystal_density_diffrn    4.448
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       slice
_exptl_crystal_F_000             342
_exptl_crystal_size_max          0.2500
_exptl_crystal_size_mid          0.1800
_exptl_crystal_size_min          0.0500
_refine_diff_density_max         0.702
_refine_diff_density_min         -0.916
_refine_diff_density_rms         0.200
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.971
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     59
_refine_ls_number_reflns         634
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.971
_refine_ls_R_factor_all          0.0243
_refine_ls_R_factor_gt           0.0222
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0192P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0489
_refine_ls_wR_factor_ref         0.0493
_reflns_number_gt                558
_reflns_number_total             634
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c6dt04750e2.cif
_cod_data_source_block           x
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7042557--7042558.cif.
;
_cod_original_sg_symbol_H-M      'P 2/c'
_cod_database_code               7042557
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Te1 Te 0.5000 0.25660(3) 0.7500 0.00566(13) Uani 1 2 d S
Co1 Co 0.5000 0.58532(6) 0.7500 0.0077(2) Uani 1 2 d S
O1 O 0.2988(5) 0.4093(2) 0.5308(5) 0.0077(6) Uani 1 1 d .
O2 O 0.6986(5) 0.2679(2) 0.5231(5) 0.0082(6) Uani 1 1 d .
O3 O 0.2816(5) 0.1184(3) 0.5415(5) 0.0082(5) Uani 1 1 d .
Na1 Na 0.5000 0.08151(18) 0.2500 0.0050(5) Uani 1 2 d S
Na2 Na 0.0000 0.5721(2) 0.2500 0.0115(5) Uani 1 2 d S
Na3 Na 0.0000 0.2577(2) 0.2500 0.0179(6) Uani 1 2 d S
Na4 Na 0.0000 0.0820(2) 0.7500 0.0189(6) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Te1 O3 92.65(16) . 2_656
O3 Te1 O2 93.12(12) . .
O3 Te1 O2 91.28(12) 2_656 .
O3 Te1 O2 91.28(12) . 2_656
O3 Te1 O2 93.12(12) 2_656 2_656
O2 Te1 O2 173.62(14) . 2_656
O3 Te1 O1 174.96(9) . 2_656
O3 Te1 O1 90.83(12) 2_656 2_656
O2 Te1 O1 90.44(12) . 2_656
O2 Te1 O1 84.89(12) 2_656 2_656
O3 Te1 O1 90.83(12) . .
O3 Te1 O1 174.96(9) 2_656 .
O2 Te1 O1 84.89(12) . .
O2 Te1 O1 90.44(12) 2_656 .
O1 Te1 O1 85.93(15) 2_656 .
O3 Te1 Na1 46.67(8) . .
O3 Te1 Na1 88.20(9) 2_656 .
O2 Te1 Na1 46.81(8) . .
O2 Te1 Na1 137.92(8) 2_656 .
O1 Te1 Na1 137.17(8) 2_656 .
O1 Te1 Na1 91.54(9) . .
O3 Te1 Na1 88.20(9) . 1_556
O3 Te1 Na1 46.67(8) 2_656 1_556
O2 Te1 Na1 137.92(8) . 1_556
O2 Te1 Na1 46.81(8) 2_656 1_556
O1 Te1 Na1 91.54(9) 2_656 1_556
O1 Te1 Na1 137.17(8) . 1_556
Na1 Te1 Na1 117.40(7) . 1_556
O3 Te1 Na1 46.33(8) . 3_656
O3 Te1 Na1 46.33(8) 2_656 3_656
O2 Te1 Na1 93.19(7) . 3_656
O2 Te1 Na1 93.19(7) 2_656 3_656
O1 Te1 Na1 137.03(7) 2_656 3_656
O1 Te1 Na1 137.03(7) . 3_656
Na1 Te1 Na1 58.70(4) . 3_656
Na1 Te1 Na1 58.70(4) 1_556 3_656
O3 Te1 Na3 136.48(9) . 1_656
O3 Te1 Na3 43.89(9) 2_656 1_656
O2 Te1 Na3 90.60(10) . 1_656
O2 Te1 Na3 89.38(10) 2_656 1_656
O1 Te1 Na3 46.94(8) 2_656 1_656
O1 Te1 Na3 132.68(8) . 1_656
Na1 Te1 Na3 118.55(5) . 1_656
Na1 Te1 Na3 61.67(5) 1_556 1_656
Na1 Te1 Na3 90.19(4) 3_656 1_656
O3 Te1 Na3 43.89(9) . .
O3 Te1 Na3 136.48(9) 2_656 .
O2 Te1 Na3 89.38(10) . .
O2 Te1 Na3 90.60(10) 2_656 .
O1 Te1 Na3 132.68(8) 2_656 .
O1 Te1 Na3 46.94(8) . .
Na1 Te1 Na3 61.67(5) . .
Na1 Te1 Na3 118.55(5) 1_556 .
Na1 Te1 Na3 90.19(4) 3_656 .
Na3 Te1 Na3 179.63(7) 1_656 .
O3 Te1 Na2 137.30(8) . 3_666
O3 Te1 Na2 87.33(10) 2_656 3_666
O2 Te1 Na2 44.23(8) . 3_666
O2 Te1 Na2 131.39(8) 2_656 3_666
O1 Te1 Na2 46.51(8) 2_656 3_666
O1 Te1 Na2 87.64(9) . 3_666
Na1 Te1 Na2 90.69(4) . 3_666
Na1 Te1 Na2 120.39(2) 1_556 3_666
Na1 Te1 Na2 119.89(4) 3_656 3_666
Na3 Te1 Na2 58.72(5) 1_656 3_666
Na3 Te1 Na2 121.06(5) . 3_666
O2 Co1 O2 95.76(14) 4_566 3_666
O2 Co1 O1 169.07(10) 4_566 .
O2 Co1 O1 93.52(11) 3_666 .
O2 Co1 O1 93.52(11) 4_566 2_656
O2 Co1 O1 169.07(10) 3_666 2_656
O1 Co1 O1 77.89(14) . 2_656
O2 Co1 O1 76.37(12) 4_566 4_566
O2 Co1 O1 101.81(11) 3_666 4_566
O1 Co1 O1 96.09(10) . 4_566
O1 Co1 O1 85.98(11) 2_656 4_566
O2 Co1 O1 101.81(11) 4_566 3_666
O2 Co1 O1 76.37(12) 3_666 3_666
O1 Co1 O1 85.98(11) . 3_666
O1 Co1 O1 96.09(10) 2_656 3_666
O1 Co1 O1 177.34(12) 4_566 3_666
O2 Co1 Na1 47.88(7) 4_566 3_666
O2 Co1 Na1 47.88(7) 3_666 3_666
O1 Co1 Na1 141.05(7) . 3_666
O1 Co1 Na1 141.05(7) 2_656 3_666
O1 Co1 Na1 88.67(6) 4_566 3_666
O1 Co1 Na1 88.67(6) 3_666 3_666
O2 Co1 Na3 54.60(8) 4_566 3_666
O2 Co1 Na3 87.37(9) 3_666 3_666
O1 Co1 Na3 131.83(8) . 3_666
O1 Co1 Na3 93.32(9) 2_656 3_666
O1 Co1 Na3 130.86(7) 4_566 3_666
O1 Co1 Na3 47.48(7) 3_666 3_666
Na1 Co1 Na3 62.22(4) 3_666 3_666
O2 Co1 Na3 87.37(9) 4_566 3_566
O2 Co1 Na3 54.60(8) 3_666 3_566
O1 Co1 Na3 93.32(9) . 3_566
O1 Co1 Na3 131.83(8) 2_656 3_566
O1 Co1 Na3 47.48(7) 4_566 3_566
O1 Co1 Na3 130.86(7) 3_666 3_566
Na1 Co1 Na3 62.22(4) 3_666 3_566
Na3 Co1 Na3 124.45(9) 3_666 3_566
O2 Co1 Na2 125.43(8) 4_566 3_566
O2 Co1 Na2 92.67(9) 3_666 3_566
O1 Co1 Na2 48.13(8) . 3_566
O1 Co1 Na2 86.63(9) 2_656 3_566
O1 Co1 Na2 49.17(7) 4_566 3_566
O1 Co1 Na2 132.49(7) 3_666 3_566
Na1 Co1 Na2 117.84(4) 3_666 3_566
Na3 Co1 Na2 179.94(4) 3_666 3_566
Na3 Co1 Na2 55.61(7) 3_566 3_566
O2 Co1 Na2 92.67(9) 4_566 3_666
O2 Co1 Na2 125.43(8) 3_666 3_666
O1 Co1 Na2 86.63(9) . 3_666
O1 Co1 Na2 48.13(8) 2_656 3_666
O1 Co1 Na2 132.49(7) 4_566 3_666
O1 Co1 Na2 49.17(7) 3_666 3_666
Na1 Co1 Na2 117.84(4) 3_666 3_666
Na3 Co1 Na2 55.61(7) 3_666 3_666
Na3 Co1 Na2 179.94(4) 3_566 3_666
Na2 Co1 Na2 124.33(9) 3_566 3_666
O2 Co1 Na2 138.53(8) 4_566 .
O2 Co1 Na2 45.83(8) 3_666 .
O1 Co1 Na2 48.90(8) . .
O1 Co1 Na2 126.62(8) 2_656 .
O1 Co1 Na2 94.64(10) 4_566 .
O1 Co1 Na2 85.47(10) 3_666 .
Na1 Co1 Na2 92.24(4) 3_666 .
Na3 Co1 Na2 123.10(5) 3_666 .
Na3 Co1 Na2 59.36(5) 3_566 .
Na2 Co1 Na2 56.92(5) 3_566 .
Na2 Co1 Na2 120.62(5) 3_666 .
Te1 O1 Co1 98.09(12) . .
Te1 O1 Co1 96.46(11) . 3_666
Co1 O1 Co1 94.02(11) . 3_666
Te1 O1 Na3 95.16(11) . .
Co1 O1 Na3 165.93(13) . .
Co1 O1 Na3 89.16(10) 3_666 .
Te1 O1 Na2 96.38(11) . 3_566
Co1 O1 Na2 89.69(10) . 3_566
Co1 O1 Na2 166.00(13) 3_666 3_566
Na3 O1 Na2 84.13(10) . 3_566
Te1 O1 Na2 171.41(13) . .
Co1 O1 Na2 89.18(10) . .
Co1 O1 Na2 87.55(10) 3_666 .
Na3 O1 Na2 77.25(11) . .
Na2 O1 Na2 79.00(10) 3_566 .
Te1 O2 Co1 101.98(13) . 3_666
Te1 O2 Na2 100.07(11) . 3_666
Co1 O2 Na2 94.05(11) 3_666 3_666
Te1 O2 Na1 96.24(11) . .
Co1 O2 Na1 91.08(11) 3_666 .
Na2 O2 Na1 161.48(13) 3_666 .
Te1 O2 Na4 95.12(11) . 1_655
Co1 O2 Na4 162.52(13) 3_666 1_655
Na2 O2 Na4 86.44(11) 3_666 1_655
Na1 O2 Na4 83.41(10) . 1_655
Te1 O2 Na3 172.91(13) . 1_655
Co1 O2 Na3 85.07(10) 3_666 1_655
Na2 O2 Na3 79.98(10) 3_666 1_655
Na1 O2 Na3 82.76(9) . 1_655
Na4 O2 Na3 77.80(9) 1_655 1_655
Te1 O3 Na3 100.56(13) . .
Te1 O3 Na4 103.22(12) . .
Na3 O3 Na4 89.74(11) . .
Te1 O3 Na1 97.77(12) . 3_656
Na3 O3 Na1 161.47(13) . 3_656
Na4 O3 Na1 88.69(10) . 3_656
Te1 O3 Na1 97.23(12) . .
Na3 O3 Na1 90.89(10) . .
Na4 O3 Na1 159.06(14) . .
Na1 O3 Na1 84.12(10) 3_656 .
Te1 O3 Na4 176.74(13) . 3_556
Na3 O3 Na4 81.66(10) . 3_556
Na4 O3 Na4 79.10(10) . 3_556
Na1 O3 Na4 79.91(10) 3_656 3_556
Na1 O3 Na4 80.29(9) . 3_556
O2 Na1 O2 82.08(14) . 2_655
O2 Na1 O3 169.61(9) . 4
O2 Na1 O3 103.78(10) 2_655 4
O2 Na1 O3 103.78(10) . 3_656
O2 Na1 O3 169.61(9) 2_655 3_656
O3 Na1 O3 71.81(14) 4 3_656
O2 Na1 O3 72.79(11) . .
O2 Na1 O3 94.05(11) 2_655 .
O3 Na1 O3 98.01(11) 4 .
O3 Na1 O3 95.88(10) 3_656 .
O2 Na1 O3 94.05(11) . 2_655
O2 Na1 O3 72.79(11) 2_655 2_655
O3 Na1 O3 95.88(10) 4 2_655
O3 Na1 O3 98.01(11) 3_656 2_655
O3 Na1 O3 162.83(15) . 2_655
O2 Na1 Na1 141.85(8) . 3_655
O2 Na1 Na1 87.52(8) 2_655 3_655
O3 Na1 Na1 47.98(7) 4 3_655
O3 Na1 Na1 82.61(10) 3_656 3_655
O3 Na1 Na1 144.84(9) . 3_655
O3 Na1 Na1 47.90(7) 2_655 3_655
O2 Na1 Na1 87.52(8) . 3_656
O2 Na1 Na1 141.85(8) 2_655 3_656
O3 Na1 Na1 82.61(10) 4 3_656
O3 Na1 Na1 47.98(7) 3_656 3_656
O3 Na1 Na1 47.90(7) . 3_656
O3 Na1 Na1 144.84(9) 2_655 3_656
Na1 Na1 Na1 120.97(12) 3_655 3_656
O2 Na1 Co1 41.04(7) . 3_666
O2 Na1 Co1 41.04(7) 2_655 3_666
O3 Na1 Co1 144.09(7) 4 3_666
O3 Na1 Co1 144.09(7) 3_656 3_666
O3 Na1 Co1 81.42(8) . 3_666
O3 Na1 Co1 81.42(8) 2_655 3_666
Na1 Na1 Co1 119.52(6) 3_655 3_666
Na1 Na1 Co1 119.52(6) 3_656 3_666
O2 Na1 Te1 36.95(7) . .
O2 Na1 Te1 90.89(9) 2_655 .
O3 Na1 Te1 133.34(7) 4 .
O3 Na1 Te1 98.94(7) 3_656 .
O3 Na1 Te1 36.09(7) . .
O3 Na1 Te1 130.77(9) 2_655 .
Na1 Na1 Te1 178.22(8) 3_655 .
Na1 Na1 Te1 60.82(6) 3_656 .
Co1 Na1 Te1 58.70(4) 3_666 .
O2 Na1 Te1 90.89(9) . 1_554
O2 Na1 Te1 36.95(7) 2_655 1_554
O3 Na1 Te1 98.94(7) 4 1_554
O3 Na1 Te1 133.34(7) 3_656 1_554
O3 Na1 Te1 130.77(9) . 1_554
O3 Na1 Te1 36.09(7) 2_655 1_554
Na1 Na1 Te1 60.82(6) 3_655 1_554
Na1 Na1 Te1 178.22(8) 3_656 1_554
Co1 Na1 Te1 58.70(4) 3_666 1_554
Te1 Na1 Te1 117.40(7) . 1_554
O2 Na1 Te1 138.96(7) . 3_656
O2 Na1 Te1 138.96(7) 2_655 3_656
O3 Na1 Te1 35.91(7) 4 3_656
O3 Na1 Te1 35.91(7) 3_656 3_656
O3 Na1 Te1 98.58(8) . 3_656
O3 Na1 Te1 98.58(8) 2_655 3_656
Na1 Na1 Te1 60.48(6) 3_655 3_656
Na1 Na1 Te1 60.48(6) 3_656 3_656
Co1 Na1 Te1 180.0 3_666 3_656
Te1 Na1 Te1 121.30(4) . 3_656
Te1 Na1 Te1 121.30(4) 1_554 3_656
O2 Na2 O2 97.85(15) 3_666 4_465
O2 Na2 O1 72.60(11) 3_666 4_565
O2 Na2 O1 101.63(11) 4_465 4_565
O2 Na2 O1 101.63(11) 3_666 3_566
O2 Na2 O1 72.60(11) 4_465 3_566
O1 Na2 O1 171.49(14) 4_565 3_566
O2 Na2 O1 173.23(9) 3_666 2
O2 Na2 O1 81.07(10) 4_465 2
O1 Na2 O1 101.00(10) 4_565 2
O1 Na2 O1 84.48(11) 3_566 2
O2 Na2 O1 81.07(10) 3_666 .
O2 Na2 O1 173.23(9) 4_465 .
O1 Na2 O1 84.48(11) 4_565 .
O1 Na2 O1 101.00(10) 3_566 .
O1 Na2 O1 100.77(14) 2 .
O2 Na2 Na3 131.07(7) 3_666 .
O2 Na2 Na3 131.07(8) 4_465 .
O1 Na2 Na3 94.25(7) 4_565 .
O1 Na2 Na3 94.25(7) 3_566 .
O1 Na2 Na3 50.39(7) 2 .
O1 Na2 Na3 50.39(7) . .
O2 Na2 Na2 123.64(8) 3_666 3_565
O2 Na2 Na2 91.96(8) 4_465 3_565
O1 Na2 Na2 51.09(6) 4_565 3_565
O1 Na2 Na2 133.99(8) 3_566 3_565
O1 Na2 Na2 49.92(8) 2 3_565
O1 Na2 Na2 94.20(10) . 3_565
Na3 Na2 Na2 63.41(7) . 3_565
O2 Na2 Na2 91.96(8) 3_666 3_566
O2 Na2 Na2 123.64(8) 4_465 3_566
O1 Na2 Na2 133.99(8) 4_565 3_566
O1 Na2 Na2 51.09(6) 3_566 3_566
O1 Na2 Na2 94.20(10) 2 3_566
O1 Na2 Na2 49.92(8) . 3_566
Na3 Na2 Na2 63.41(7) . 3_566
Na2 Na2 Na2 126.82(14) 3_565 3_566
O2 Na2 Na3 54.23(8) 3_666 3_566
O2 Na2 Na3 85.17(9) 4_465 3_566
O1 Na2 Na3 126.79(8) 4_565 3_566
O1 Na2 Na3 47.59(7) 3_566 3_566
O1 Na2 Na3 132.04(7) 2 3_566
O1 Na2 Na3 88.82(8) . 3_566
Na3 Na2 Na3 120.59(5) . 3_566
Na2 Na2 Na3 176.00(10) 3_565 3_566
Na2 Na2 Na3 57.18(7) 3_566 3_566
O2 Na2 Na3 85.17(9) 3_666 3_565
O2 Na2 Na3 54.23(8) 4_465 3_565
O1 Na2 Na3 47.59(7) 4_565 3_565
O1 Na2 Na3 126.79(8) 3_566 3_565
O1 Na2 Na3 88.82(8) 2 3_565
O1 Na2 Na3 132.04(7) . 3_565
Na3 Na2 Na3 120.59(5) . 3_565
Na2 Na2 Na3 57.18(7) 3_565 3_565
Na2 Na2 Na3 176.00(10) 3_566 3_565
Na3 Na2 Na3 118.82(10) 3_566 3_565
O2 Na2 Co1 143.23(7) 3_666 3_566
O2 Na2 Co1 79.20(9) 4_465 3_566
O1 Na2 Co1 144.13(8) 4_565 3_566
O1 Na2 Co1 42.18(7) 3_566 3_566
O1 Na2 Co1 43.28(7) 2 3_566
O1 Na2 Co1 97.62(10) . 3_566
Na3 Na2 Co1 62.16(4) . 3_566
Na2 Na2 Co1 93.13(6) 3_565 3_566
Na2 Na2 Co1 61.80(4) 3_566 3_566
Na3 Na2 Co1 89.08(3) 3_566 3_566
Na3 Na2 Co1 119.43(2) 3_565 3_566
O3 Na3 O3 108.59(16) 2 .
O3 Na3 O1 176.32(8) 2 .
O3 Na3 O1 73.43(11) . .
O3 Na3 O1 73.43(11) 2 2
O3 Na3 O1 176.32(8) . 2
O1 Na3 O1 104.73(15) . 2
O3 Na3 O2 93.42(10) 2 2_655
O3 Na3 O2 89.07(10) . 2_655
O1 Na3 O2 83.48(10) . 2_655
O1 Na3 O2 93.91(11) 2 2_655
O3 Na3 O2 89.07(10) 2 1_455
O3 Na3 O2 93.42(10) . 1_455
O1 Na3 O2 93.91(11) . 1_455
O1 Na3 O2 83.48(10) 2 1_455
O2 Na3 O2 175.75(13) 2_655 1_455
O3 Na3 Na2 125.71(8) 2 .
O3 Na3 Na2 125.71(8) . .
O1 Na3 Na2 52.36(7) . .
O1 Na3 Na2 52.36(7) 2 .
O2 Na3 Na2 87.87(7) 2_655 .
O2 Na3 Na2 87.87(7) 1_455 .
O3 Na3 Na2 134.48(7) 2 3_566
O3 Na3 Na2 83.88(8) . 3_566
O1 Na3 Na2 48.27(7) . 3_566
O1 Na3 Na2 92.52(9) 2 3_566
O2 Na3 Na2 131.25(8) 2_655 3_566
O2 Na3 Na2 45.80(6) 1_455 3_566
Na2 Na3 Na2 59.41(5) . 3_566
O3 Na3 Na2 83.88(8) 2 3_565
O3 Na3 Na2 134.48(7) . 3_565
O1 Na3 Na2 92.52(9) . 3_565
O1 Na3 Na2 48.27(7) 2 3_565
O2 Na3 Na2 45.80(6) 2_655 3_565
O2 Na3 Na2 131.25(8) 1_455 3_565
Na2 Na3 Na2 59.41(5) . 3_565
Na2 Na3 Na2 118.82(10) 3_566 3_565
O3 Na3 Co1 133.37(7) 2 3_666
O3 Na3 Co1 81.80(8) . 3_666
O1 Na3 Co1 43.36(7) . 3_666
O1 Na3 Co1 99.09(10) 2 3_666
O2 Na3 Co1 40.33(6) 2_655 3_666
O2 Na3 Co1 136.70(8) 1_455 3_666
Na2 Na3 Co1 62.22(4) . 3_666
Na2 Na3 Co1 90.96(5) 3_566 3_666
Na2 Na3 Co1 60.59(3) 3_565 3_666
O3 Na3 Co1 81.80(8) 2 3_566
O3 Na3 Co1 133.37(7) . 3_566
O1 Na3 Co1 99.09(10) . 3_566
O1 Na3 Co1 43.36(7) 2 3_566
O2 Na3 Co1 136.70(8) 2_655 3_566
O2 Na3 Co1 40.33(6) 1_455 3_566
Na2 Na3 Co1 62.22(4) . 3_566
Na2 Na3 Co1 60.59(3) 3_566 3_566
Na2 Na3 Co1 90.96(5) 3_565 3_566
Co1 Na3 Co1 124.45(9) 3_666 3_566
O3 Na3 Na4 45.23(7) 2 1_554
O3 Na3 Na4 95.53(9) . 1_554
O1 Na3 Na4 132.06(7) . 1_554
O1 Na3 Na4 88.06(8) 2 1_554
O2 Na3 Na4 49.21(6) 2_655 1_554
O2 Na3 Na4 133.79(8) 1_455 1_554
Na2 Na3 Na4 121.39(5) . 1_554
Na2 Na3 Na4 179.20(7) 3_566 1_554
Na2 Na3 Na4 61.98(7) 3_565 1_554
Co1 Na3 Na4 89.48(3) 3_666 1_554
Co1 Na3 Na4 119.64(2) 3_566 1_554
O3 Na4 O3 162.51(17) . 2_556
O3 Na4 O2 70.28(11) . 2_656
O3 Na4 O2 96.95(11) 2_556 2_656
O3 Na4 O2 96.95(11) . 1_455
O3 Na4 O2 70.28(11) 2_556 1_455
O2 Na4 O2 89.27(14) 2_656 1_455
O3 Na4 O3 100.90(10) . 3_556
O3 Na4 O3 91.68(11) 2_556 3_556
O2 Na4 O3 171.19(8) 2_656 3_556
O2 Na4 O3 91.99(10) 1_455 3_556
O3 Na4 O3 91.68(11) . 4_556
O3 Na4 O3 100.90(10) 2_556 4_556
O2 Na4 O3 91.99(10) 2_656 4_556
O2 Na4 O3 171.19(8) 1_455 4_556
O3 Na4 O3 88.09(13) 3_556 4_556
O3 Na4 Na4 55.70(7) . 3_556
O3 Na4 Na4 135.56(8) 2_556 3_556
O2 Na4 Na4 125.99(8) 2_656 3_556
O2 Na4 Na4 96.70(8) 1_455 3_556
O3 Na4 Na4 45.20(7) 3_556 3_556
O3 Na4 Na4 89.61(10) 4_556 3_556
O3 Na4 Na4 135.56(8) . 3_557
O3 Na4 Na4 55.70(7) 2_556 3_557
O2 Na4 Na4 96.70(8) 2_656 3_557
O2 Na4 Na4 125.99(8) 1_455 3_557
O3 Na4 Na4 89.61(10) 3_556 3_557
O3 Na4 Na4 45.20(7) 4_556 3_557
Na4 Na4 Na4 120.67(14) 3_556 3_557
O3 Na4 Na3 123.25(9) . 1_556
O3 Na4 Na3 45.04(7) 2_556 1_556
O2 Na4 Na3 52.99(7) 2_656 1_556
O2 Na4 Na3 81.99(9) 1_455 1_556
O3 Na4 Na3 135.82(6) 3_556 1_556
O3 Na4 Na3 91.81(8) 4_556 1_556
Na4 Na4 Na3 178.27(10) 3_556 1_556
Na4 Na4 Na3 61.05(7) 3_557 1_556
O3 Na4 Na3 45.04(7) . .
O3 Na4 Na3 123.25(9) 2_556 .
O2 Na4 Na3 81.99(9) 2_656 .
O2 Na4 Na3 52.99(7) 1_455 .
O3 Na4 Na3 91.81(8) 3_556 .
O3 Na4 Na3 135.82(7) 4_556 .
Na4 Na4 Na3 61.05(7) 3_556 .
Na4 Na4 Na3 178.27(10) 3_557 .
Na3 Na4 Na3 117.22(10) 1_556 .
O3 Na4 Na1 98.00(9) . 1_455
O3 Na4 Na1 82.03(9) 2_556 1_455
O2 Na4 Na1 133.65(10) 2_656 1_455
O2 Na4 Na1 46.51(7) 1_455 1_455
O3 Na4 Na1 45.89(7) 3_556 1_455
O3 Na4 Na1 133.94(10) 4_556 1_455
Na4 Na4 Na1 60.99(5) 3_556 1_455
Na4 Na4 Na1 118.92(6) 3_557 1_455
Na3 Na4 Na1 118.46(6) 1_556 1_455
Na3 Na4 Na1 61.64(5) . 1_455
O3 Na4 Na1 82.03(9) . 1_556
O3 Na4 Na1 98.00(9) 2_556 1_556
O2 Na4 Na1 46.51(7) 2_656 1_556
O2 Na4 Na1 133.65(10) 1_455 1_556
O3 Na4 Na1 133.94(9) 3_556 1_556
O3 Na4 Na1 45.89(7) 4_556 1_556
Na4 Na4 Na1 118.92(6) 3_556 1_556
Na4 Na4 Na1 60.99(5) 3_557 1_556
Na3 Na4 Na1 61.64(5) 1_556 1_556
Na3 Na4 Na1 118.46(6) . 1_556
Na1 Na4 Na1 179.83(9) 1_455 1_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Te1 O3 1.906(3) .
Te1 O3 1.906(3) 2_656
Te1 O2 1.941(3) .
Te1 O2 1.941(3) 2_656
Te1 O1 1.988(3) 2_656
Te1 O1 1.988(3) .
Te1 Na1 3.210(2) .
Te1 Na1 3.210(2) 1_556
Te1 Na1 3.220(3) 3_656
Te1 Na3 3.2232(19) 1_656
Te1 Na3 3.2232(19) .
Te1 Na2 3.274(2) 3_666
Co1 O2 2.084(3) 4_566
Co1 O2 2.084(3) 3_666
Co1 O1 2.155(3) .
Co1 O1 2.155(3) 2_656
Co1 O1 2.203(3) 4_566
Co1 O1 2.203(3) 3_666
Co1 Na1 3.173(3) 3_666
Co1 Na3 3.208(2) 3_666
Co1 Na3 3.208(2) 3_566
Co1 Na2 3.210(2) 3_566
Co1 Na2 3.210(2) 3_666
Co1 Na2 3.2257(19) .
O1 Co1 2.203(3) 3_666
O1 Na3 2.365(3) .
O1 Na2 2.390(3) 3_566
O1 Na2 2.431(3) .
O2 Co1 2.084(3) 3_666
O2 Na2 2.319(3) 3_666
O2 Na1 2.354(3) .
O2 Na4 2.489(3) 1_655
O2 Na3 2.625(3) 1_655
O3 Na3 2.273(3) .
O3 Na4 2.281(3) .
O3 Na1 2.351(3) 3_656
O3 Na1 2.354(3) .
O3 Na4 2.655(3) 3_556
Na1 O2 2.354(3) 2_655
Na1 O3 2.351(3) 4
Na1 O3 2.351(3) 3_656
Na1 O3 2.354(3) 2_655
Na1 Na1 3.152(2) 3_655
Na1 Na1 3.152(2) 3_656
Na1 Co1 3.173(3) 3_666
Na1 Te1 3.210(2) 1_554
Na1 Te1 3.220(3) 3_656
Na2 O2 2.319(3) 3_666
Na2 O2 2.319(3) 4_465
Na2 O1 2.390(3) 4_565
Na2 O1 2.390(3) 3_566
Na2 O1 2.431(3) 2
Na2 Na3 2.994(4) .
Na2 Na2 3.067(3) 3_565
Na2 Na2 3.067(3) 3_566
Na2 Na3 3.186(2) 3_566
Na2 Na3 3.186(2) 3_565
Na2 Co1 3.210(2) 3_566
Na3 O3 2.273(3) 2
Na3 O1 2.365(3) 2
Na3 O2 2.625(3) 2_655
Na3 O2 2.625(3) 1_455
Na3 Na2 3.186(2) 3_566
Na3 Na2 3.186(2) 3_565
Na3 Co1 3.208(2) 3_666
Na3 Co1 3.208(2) 3_566
Na3 Na4 3.213(2) 1_554
Na4 O3 2.281(3) 2_556
Na4 O2 2.489(3) 2_656
Na4 O2 2.489(3) 1_455
Na4 O3 2.655(3) 3_556
Na4 O3 2.655(3) 4_556
Na4 Na4 3.156(3) 3_556
Na4 Na4 3.156(3) 3_557
Na4 Na3 3.213(2) 1_556
Na4 Na1 3.2232(19) 1_455
Na4 Na1 3.2232(19) 1_556
